Stereolithography Cure Process Modeling Using Acrylate Resin
Yanyan Tang†, Clifford L. Henderson†, John Muzzy†, David W. Rosen*
† School of Chemical & Biomolecular Engineering, 311 Ferst Drive, N.W., Georgia Institute of
Technology, Atlanta, GA 30332-0100
*Corresponding author; School of Mechanical Engineering, 813 Ferst Drive, N.W., Georgia
Institute of Technology, Atlanta, GA 30332-0405; Email: firstname.lastname@example.org
Reviewed, accepted September 1, 2004
In this paper, a complex stereolithography (SL) cure process model is presented that
incorporates transient thermal and chemical effects which influence final part shape and
properties. The model incorporates photopolymerization, mass diffusion, and heat transfer.
Material properties are characterized and a comprehensive kinetic model parameterized for a
model compound system. SL process simulations are performed using finite element methods
with the software package FEMLAB, and validated by the capability of predicting the fabricated
part dimensions. A degree of cure (DOC) threshold model is proposed which can predict the cure
line size within 15% error, comparing with 30% prediction error by the exposure threshold
model currently used in SL. Furthermore, through the sensitivity analysis conducted by the
process model presented here, the sensitive parameters are identified and the SL bath
temperature, photointiator absorptivity and concentration are found to be the most sensitive
factors that affect the SL fabrication results. The sensitive variables will be the focus of further
research meant to improve SL process speed and resolution.
In the stereolithography (SL) process, parts are fabricated in a layer-by-layer manner by
curing photopolymer resins with a UV laser. For some applications, the SL process requires
improvements in speed and resolution, but it is not clear that both can be improved
simultaneously. A better understanding of the SL process is needed in order to improve the
technology. Being able to simulate and predict part shape, build time, and potential difficulties
would be very beneficial. To accomplish this, a more complete model of SL cure is needed .
Furthermore, improvements to SL machines can be investigated to determine their impact on
building speed, resolution, and other concerns.
Current models of the SL process assume that the extent of resin curing is a function of only
the amount of exposure to UV radiation . They utilize a threshold model that assumes a dose
E(x,y,z) that is greater than a minimum “critical exposure,” Ec, causes the resin to solidify at
point (x,y,z). This is a gross oversimplification of the process that ignores important transient,
thermal, and chemical effects. SL cure is a time-varying process that is governed by complex,
exothermic chemical reactions that have multiple reaction pathways. A more complete model is
needed that accounts for these effects.
In this paper, a more complex SL cure model is presented that captures effects that are
ignored in the threshold model. It incorporates heat transfer, mass transfer, and reaction kinetics,
and thus simulates the variation of temperature and material properties during the SL curing
process. It is important to model the transient 3-D distribution of temperature, since temperature
influences reaction rates and, if high enough, can cause thermal curing. With the SL cure model
presented here, it is possible to investigate the spatial and temporal distributions of monomer and
polymer concentrations, molecular weight, cross-link density, and degree of cure, which are
necessary to characterize the cured part. This paper presents that the size of the cured part can be
predicted from the monomer conversion profile.
The SL cure model is formulated as a set of partial differential equations, with initial
conditions specified based on the chemistry and physics of laser exposure and photoinitiation.
This model is then solved using the finite element method with the software package FEMLAB.
Numerical results are compared with experimental measurements and it is shown that from the
degree of cure profile, the cured part size upon variation of process or material parameters can be
The simplest case of complex laser drawing patterns in SL apparatus is that the laser moves
along one direction and draws a single vector scan line. The cured shape upon a single laser
drawn line is a parabolic cylinder , as shown in Figure 1, where the x axis is the laser drawing
direction. Considering the repetition of the parabolic plane along the x axis and its symmetry
about the x-z plane, a rectangular domain in Cartesian coordinates (Figure 2) was established to
simulate the resin cure behaviour during the single-line drawing process. The shaded region is
where the temperature or concentrations vary, the size of which increases with time as heat
conduction and/or molecular diffusion continues . The domain is chosen to be large enough to
ensure ambient temperature and concentrations outside the rectangle at any time.
Figure 1 SL cured shape upon a single laser drawn line
Figure 2 SL process modelling domain for single laser drawn line
Mass transfer by diffusion and heat transfer by conduction are the two transport phenomena
occurring in the SL cure process. Equations (1)-(3) describe the energy balance, mass balance for
monomer, and mass balance for the polymeric radicals (including monomer radicals),
The source terms PP RH∆ , - PR , and - tR are dependent on the photopolymerization kinetics of
the resin, which will be discussed later. The terms containing x variations can be removed
neglecting property variations in the scanning direction (x axis). The corresponding initial and
boundary conditions are as follows:
twy, C zQQ
tzC, w yQQ
b tzC, y
where Q represents T, [M], or [P• ], Cd is the cure depth, maximum depth of the polymerized
area, and w0 is the laser beam radius. The domain size can be initially set based on the Cd and w0
values and adjusted later according to the simulation results. Note that for both temperature and
monomer concentration, 0][ QQ i = , but for radical concentration, 0=][ 0Q and 0][ QQ i ≠ , where
iQ][ will be addressed soon. For the temperature condition at z=0 boundary, heat transfer with
the natural air environment was considered, and thus temperature condition (d) in Equation (4)
Tk h T T
∂ = −
at z = 0, 0 ≤ y ≤ 5w0, t ≥ 0 (5)
where h is the heat transfer coefficient at the resin surface in the SL machine chamber, and Tinf is
the environmental temperature in the SL machine chamber.
Photopolymerization Kinetic Model
As mentioned earlier, all source terms in the balance equations are related to the kinetics of
the resin polymerization. The photocure kinetics of the resin therefore needs to be characterized.
The mechanism of radical photopolymerization can be briefly described as follows:
n PMP p Propagation
mn MPP tc +→•+• Termination by Combination
mn MMPP td +→•+• Termination by Disproportionation
where PI represents the photoinitiator, which decays to generate primary radicals ][ •R ; M stands
for monomer, which reacts with radicals to create and elongate polymer chains •nP ; these chain
radicals •nP could combine with one another and terminate to become dead polymer nM ,
which is no longer reactive.
Corresponding to the reaction mechanism, the rates of the initiation, propagation and
termination reactions are expressed as Equations (7), (8) and (9), respectively.
aii IφR = (7)
]][•[= MPkR pP (8)
2]•[= PkR tt (9)
where iφ is the initiation quantum yield, aI is the absorbed light intensity (mol/m
3-s), ]•[P is the
chain radical concentration, ][M is the monomer concentration, and pk and tk are the
propagation and terminati